Talanta 128 (2014) 9–14
Contents lists available at ScienceDirect
Talanta journal homepage: www.elsevier.com/locate/talanta
A novel strategy for synthesis of hollow gold nanosphere and its application in electrogenerated chemiluminescence glucose biosensor Xia Zhong, Ya-Qin Chai n, Ruo Yuan n Key Laboratory of Luminescence and Real-time Analysis Chemistry, Ministry of Education, College of Chemistry and Chemical Engineering, Southwest University, Chongqing 400715, PR China
art ic l e i nf o
a b s t r a c t
Article history: Received 13 December 2013 Received in revised form 21 March 2014 Accepted 29 March 2014 Available online 4 April 2014
Well-distributed hollow gold nanospheres ([email protected]
) (207 5 nm) were synthesized using the glucose oxidase (GOD) cross-linked with glutaraldehyde as a template. A glucose biosensor was prepared based on [email protected]
nanospheres for catalyzing luminol electrogenerated chemiluminescence (ECL). Firstly, chitosan was modiﬁed in a glassy carbon electrode which offered an interface of abundant amino-groups to assemble [email protected]
nanospheres. Then, glucose oxidase was adsorbed on the surface of [email protected]
nanospheres via binding interactions between Aushell and amino groups of GOD to construct a glucose biosensor. The [email protected]
nanospheres were investigated with TEM and UV–vis. The ECL behaviors of the biosensor were also investigated. Results showed that, the obtained [email protected]
nanospheres exhibited excellent catalytic effect towards the ECL of luminol-H2O2 system. The response of the prepared biosensor to glucose was linear with the glucose concentration in the range of 1.0 μM to 4.3 mM (R¼0.9923) with a detection limit of 0.3 μM (signal to noise ¼3). This ECL biosensor exhibited short response time and excellent stability for glucose. At the same time the prepared ECL biosensor showed good reproducibility, sensitivity and selectivity. & 2014 Elsevier B.V. All rights reserved.
Keywords: Electrogenerated chemiluminescence Glutaraldehyde Glucose oxidase Nanospheres Glucose
1. Introduction Electrogenerated chemiluminescence (also known as electrochemiluminescence) is the combination electrochemistry and chemiluminescence, which not only possesses the advantages of electrochemical analysis, but also exhibits many characteristics of chemiluminescence analysis . As a new electrochemical detection technology, electrogenerated chemiluminescence (ECL) is of interest to researchers due to its versatility, simpliﬁed optical setup, low background signal and high sensitivity. Electrogenerated chemiluminescence signals are usually obtained from the excited states of a luminophore generated at the electrode surface during the electrochemical reaction . Electrogenerated chemiluminescence technology has been widely applied in the ﬁeld of biotechnology, food safety and clinical diagnosis [3–5]. In recent years, some enzyme biosensors based on electrogenerated chemiluminescence also have been reported for detecting glucose, alcohol, hypoxanthine, cholesterol, choline, etc. [6–10]. Luminol (2,3-aminophthalhydrazide) has been widely used in constructing electrogenerated chemiluminescence systems because
Corresponding authors. Tel.: þ 86 23 6825 2277; fax: þ86 23 6825 4000. E-mail addresses: [email protected]
(Y.-Q. Chai), [email protected]
(R. Yuan). http://dx.doi.org/10.1016/j.talanta.2014.03.071 0039-9140/& 2014 Elsevier B.V. All rights reserved.
of its low oxidation potential, inexpensive reagent consumption and the high emission yields [11–13]. The electrogenerated chemiluminescence of luminol can be triggered by applying an appropriate positive potential to the working electrode in the presence of hydrogen peroxide (H2O2) [1,9]. Some enzymes can produce H2O2 during their substrate-speciﬁc enzymatic reaction. The intensity of the electrogenerated chemiluminescence signal is directly proportional to the concentration of H2O2 which was generated by enzymatical catalysis. Therefore, a sensitive electrogenerated chemiluminescence glucose biosensor could be designed for measurement of glucose by detecting H2O2 indirectly [14,15]. Some nanomaterials such as gold nanoparticles (AuNPs) [9,16], platinum nanoparticles , palladium nanoparticles , graphene , TiO2 nanocrystals  and quantum dots  have been used in the electrogenerated chemiluminescence system. Among these nanomaterials, gold nanoparticles have excellent catalytic performance to directly enhance the electrogenerated chemiluminescence intensity of luminol-H2O2 system [20–22]. So, gold nanoparticles can be used as the immobilization matrix for the design of a novel biosensor with enhanced analytical performance. A lot of hollow capsules nanoparticles have been synthesized and applied [23–26]. Sharma's group  has obtained hollow gold nanoparticles by leaching out silver chloride (AgCl) from [email protected]
nanoparticles with dilute ammonia solution, Jiang's group  has synthesized Polystyrene/gold core–shell
X. Zhong et al. / Talanta 128 (2014) 9–14
nanocomposites based on the method of ionic self-assembly and the in situ reduction. These preparation process of hollow gold nanoparticles were complicated. Herein, the aim of this work is to synthesize well-distributed hollow gold nanospheres encapsulating GOD ([email protected]
) (about 207 5 nm) in a simple way and develop an ECL biosensor. The prepared hollow [email protected]
nanoparticles have large surface area, high conductivity, good biocompatibility, which could effectively increase the loading of GOD and keep the biological activity of GOD. Thus, GOD molecules can exist inside and outside of the Aushell, which could effectively amplify the ECL intensity of luminol-H2O2 system. In addition, the Aushell assembling on the electrode can catalyze the electro-oxidization of luminol, and the more strong ECL signal was obtained in neutral aqueous solution. Such fabrication of biosensor exhibited short response time and excellent stability for glucose detecting. At the same time the prepared ECL biosensor showed good reproducibility, sensitivity and selectivity.
2. Experimental 2.1. Reagents and materials GOD and chitosan (CS) were obtained from Sigma Chemical Co. (St. Louis, MO, USA). Gold chloride tetrahydrate (HAuCl4 4H2O) was obtained from Sinopharm Chemical Reagent Co. Ltd. (Shanghai, China). Glutaraldehyde (GA) was purchased from Beijing Chemical Reagent Co. (Beijing, China). L-ascorbic acid (AA) was purchased from Boyi Chemical Reagent Co. (Chongqing, China). Phosphate buffer solutions (PBS) with various pH values were prepared with 0.1 M KH2PO4 and 0.1 M Na2HPO4. The supporting electrolyte was 0.1 M KCl. All chemicals were analytical grade and were used as received without further puriﬁcation. Ultrapure water was used throughout all experiments.
2.2. Apparatus The ECL emission was measured using a model MPI-A electrochemilu-minescence analyzer (Xi'an Remax Electronic Science & Technology Co. Ltd., China) with the voltage of the photomultiplier tube (PMT) set at 600 V in the detection process. Cyclic voltammetry (CV) was performed with a CHI 600D electrochemical work station (Shanghai CH Instruments Co., China). All experiments were performed with a conventional three-electrode system including a bare or modiﬁed glassy carbon electrode (GCE, Φ¼4 mm) as working electrode, a platinum wire as auxiliary electrode and a saturated calomel electrode (SCE) as reference electrode for electrochemical experiments, or Ag/AgCl electrode as a reference electrode for ECL experiments. The morphologies of the prepared of [email protected]
were tracked by transmission electron microscopy (TEM, H600, Hitachi Instrument, Japan). 2.3. Preparation of hollow gold nanospheres encapsulating GOD ([email protected]
) The hollow gold nanospheres encapsulating GOD were synthesized using GOD cross-linked with glutaraldehyde as a template. Brieﬂy, GOD cross-linked with glutaraldehyde was obtained by mixing 1.0 mL of 2 mg L 1 GOD solutions (pH 7.0) with 1.0 mL of 1.0% glutaraldehyde solution. Then, the mixture solution was placed in a refrigerator at 4 1C for 12 h. Subsequently, 0.5 mL of above mixture solution and 100 mL of 1.0% gold chloride tetrahydrate were added in 5.0 mL ultrapure water with stirring. Afterward, 0.01 M ascorbic acid (AA) was injected into the solution with droplet under agitation, and the color of solution changed to claret. In the GOD-glutaraldehyde network structure, AuCl4 can be reduced by ascorbic acid to elemental Au that could grow into hollow gold nanospheres ([email protected]
) in control. The morphology of [email protected]
was measured by TEM. The schematic diagram of the stepwise procedure of the synthesis is illustrated in Scheme 1(A).
Scheme 1. (A) Synthesized process of hollow gold nanospheres ([email protected]
); (B) Schematic description of response mechanism.
X. Zhong et al. / Talanta 128 (2014) 9–14
A glassy carbon electrode was polished with 0.3 and 0.05 mm alumina slurry to gain a slick surface, and then was ultrasonically cleaned in ethanol and water drastically. Then it was dried at room temperature. Following this pretreatment, 10 ml of CS aqueous dispersion (1.0 mg mL 1) was dropped on cleaned GCE. Then it was allowed to dry at room temperature in air. Subsequently, it was immersed in [email protected]
solution for 8 h to obtain [email protected]
/CS/GCE. Afterward, the [email protected]
/CS/GCE was immersed in GOD solution (2 mg mL 1 in PBS, pH 7.0) for another 8 h to fabricate the GOD/[email protected]
/CS/GCE. The modiﬁed process is schematically shown in Scheme 1(B). The biosensor was stored at 4 1C in a refrigerator when not in use. The probable principle of this biosensor related to the detection of glucose is also schematically shown in Scheme 1(B). The glucose in the solution reacts with the dissolved oxygen (O2) in the presence of GOD to generate gluconolactone and H2O2 (Eq. (1)). Under positive potential and with the help of Aushell, the luminol radical anion reacts with H2O2, the product of the enzymatic reaction of GOD and glucose, at the electrode surface to produce the excited state 3-aminophthalate anion, which emits an ECL emission at 425 nm (Eq. (2)). The intensity of the ECL signal is directly proportional to the concentration of H2O2 which was produced by GOD and glucose. Therefore, a sensitive ECL glucose sensor could be developed for the detection of glucose by detecting H2O2 indirectly. Based on this principle, an ECL biosensor for glucose could be fabricated. D glucose þ O2 - H2 O2 þ D gluconolactone
2H2 O2 þ luminol-3aminophthalate þ N2 þ 3H2 Oþ hv
2.4. Fabrication of the ECL biosensor
0.9 0.6 0.3 0.0 400
500 600 700 Wavelength / nm
Fig. 1. (A) TEM images of [email protected]
nanospheres (mode: Microprobe, voltage: 80 KV and current: 12.23 mA); and (B) UV–vis spectra of hollow [email protected]
3.2. Electrochemical impedance spectroscopy (EIS) and cyclic voltammetry (CV) characterization of the enzyme electrode 2.5. Measurement procedure The prepared biosensor was placed in an ECL detector cell containing 3 mL PBS with 0.1 mM luminol and different concentration of glucose to record the change of ECL signals at room temperature. The voltage of the photomultiplier tube (PMT) was set at 600 V and the applied potential was 0.2–0.8 V (vs. Ag/AgCl) with a scan rate of 100 mV s 1 in the process of detection. On increasing the glucose concentration, the ECL signals of luminol enhanced. Therefore, the changes of ECL intensity directly connected with the concentration changes of glucose.
3. Results and discussion 3.1. Characterization of the [email protected]
nanoparticles TEM technique was employed to conﬁrm the successful synthesis of the hollow nanoparticles. A typical TEM image of [email protected]
is shown in Fig. 1(A). The photograph shows that well-dispersed [email protected]
are a hollow spherical with a mean size about 20 75 nm. UV–vis absorption spectroscopy was used to further characterize the component of the hollow nanoparticles. The UV–vis absorption spectra of the [email protected]
colloidal solutions present a well-deﬁned absorption band with a maximum at the wavelength λmax ¼527 nm (Fig. 1(B)). The AuNPs are known to have an intense Plasmon absorption band in this region . Therefore, the absorption band at 527 nm arises from surface plasmon absorption of [email protected]
As expected, the results show that the prepared hollow [email protected]
was successfully prepared.
EIS was used to estimate the interfacial changes of the electrode. The semicircle diameter of impedance equals the electron transfer resistance (Ret), which lies on the electron transfer kinetics of the redox probe at the electrode interface. Fig. 2(A) shows the impedance spectrum of the modiﬁed electrode at different stages in 5.0 mM K3Fe(CN)6/K4Fe(CN)6(1:1) solution (0.1 M KCl). The Nyquist semicircle of the CS/GCE (curve b) increased dramatically when compared with the bare GCE (curve a), which indicated that CS was fabricated on the GCE. However, when hollow [email protected]
was adsorbed on the electrode, the Nyquist semicircle decreased markedly (curve c) for the reason that hollow [email protected]
could facilitate electron transfer between solution and electrode surface. When the GOD was adsorbed on [email protected]
nanoparticles of the electrode (curve d), the Nyquist semicircle increased which may be caused by the hindrance of non-conductive GOD. For the sake of giving more detailed information about the impedance of the modiﬁed electrode, a modiﬁed Randles equivalent circuit (Fig. 2(A) insert) was chosen to ﬁt the measured results. The assembly process was also afﬁrmed by CV in the potential range of 0.3 to 0.7 V in 5.0 mM K3Fe(CN)6/K4Fe(CN)6(1:1) solution (0.1 M KCl) (Fig. 2(B)). The peak current and the peak-to-peak potential distance (ΔE) of the CV curves also revealed information about the electron-transfer process. As shown in Fig. 2(B), stable and well-deﬁned redox peaks at 0.15 and 0.28 V at a scan rate of 50 mV/s were observed at bare GCE (curve a). The peak to peak separation (ΔE) is 0.13 V. When CS was deposited on GCE surface, the resulting electrode showed redox peaks at 0.04 V and 0.39 V and the ΔE¼ 0.35 V (curve b). But an obvious decrease of peak current was noticed, which was attributed to the CS blocking the redox of the electrode surface. In comparison with curve b, the
X. Zhong et al. / Talanta 128 (2014) 9–14
In order to obtain a better ECL response to glucose, the effect of medium pH on the biosensor was investigated. In this ECL system, the pH of PBS will inﬂuence the enzyme activity and ECL signal intensity. As we know, luminol generates strong chemiluminescence or ECL signals in alkaline media. However, enzyme could not maintain its biological activity in alkaline media. Considering the pH of human blood is about 7.4 and GOD can keep its activity in this pH condition. In this case, pH 7.4 was selected to ensure sensitivity and stability of the sensor.
3.4. Performance of the biosensor
Z' re / ohm
Current / A
d b 0
Potential / V Fig. 2. EIS (A) and CVs (B) of different electrodes (a) bare GCE, (b) CS/GCE, (c) [email protected]
/CS/GCE, and (d)GOD/[email protected]
/CS/GCE in 5.0 mM [Fe(CN)6]4 /3 solution (containing 0.1 M KCl) at a scan rate of 100 mV/s. Inset (A): equivalent circuit adopted to ﬁt the impedance data, (1) Rs (electrolyte resistance); (2) Zw (Warburg impedance); (3) Ret (electron-transfer resistance); (4) Cdl (double-layer capacitance).
peak currents increased and ΔE¼ 0.15 V after loading hollow [email protected]
, which contributed to the fact that nanoparticles can promote the transmission of electrons (curve c). However, after the second layer GOD were modiﬁed onto the electrode via binding interactions between nanoparticles and amino groups of GOD, a further decrease in peak current was observed and ΔE ¼0.27 V (curve d). The conclusions of CV are conﬁrmed with EIS. The above results could clearly conﬁrm the successful assembled the biosensor. The effect of variation of scan rate on electrochemical behavior of [Fe(CN)6]3 /4 (5.0 mM) in KCl aqueous solution(0.1 M) was investigated. The variation of peak current (ip) with the square root of scan rate (v1/2) was found to be linear in the investigated scan rate range of 10–300 mV/s, demonstrating that the electrochemical process is diffusion-controlled. The diffusion coefﬁcient was 1.0 10 5 cm2 s 1. 3.3. Optimum conditions of the biosensor In order to obtain the optimum performance of the prepared ECL biosensor for glucose, the concentrations of luminol in solution and adsorbing time of hollow [email protected]
with CS in electrode were studied. The result showed that the ECL intensity increased with the increase of luminol concentration, which may be because the ECL intensity is directly proportional to the quantity of luminol. Consideration of the ECL intensity and sensitivity of the glucose biosensor, herein, 0.1 mM was selected as the optimal concentration of luminol for the optimum concentration. The adsorbing amount of [email protected]
could also inﬂuence the intensity of the ECL signal. As a result, the optimum adsorbing time is 8 h which selected for the biosensor fabrication.
The ECL response of the glucose biosensor was investigated with the ECL technique under optimal experimental conditions. A comparative study was carried out by using two kinds of biosensor (Fig. 3): [email protected]
/CS/GCE (A) and GOD/[email protected]
/CS/GCE (B). With the increasing concentration of glucose, the ECL intensity of the two kinds of biosensor is increased. The inset displays the calibration plots of the two kinds of sensor for glucose determination. For [email protected]
/CS/GCE, the ECL signals linearly increases in the range of 10 μM–3.28 mM, with a detection limit of 3 μM at the signal-to-noise ratio of 3. The regression equation was I (a.u.) ¼ 0.229 103c (mM) þ 102.06 with a correlation coefﬁcient of 0.9913. The result showed the GOD inside of [email protected]
still have its biological activity and can oxidize glucose to produce H2O2. The intensity of the ECL signal is directly proportional to the concentration of H2O2 which was produced by GOD and glucose. For GOD/[email protected]
/CS/GCE, the ECL signals increased linearly in the range of 1.0 μM–4.3 mM with a detection
ECL Intensity / a.u
800 600 400 200
200 0 12
ECL Intensity / a.u
ECL Intensity / a.u
ECL Intensity / a.u
Z'' im / ohm
12000 8000 4000 0 0
Time/s Fig. 3. ECL responses of [email protected]
/CS/GCE (A) in the presence of 0.01, 0.02, 0.08, 0.18, 0.28, 1.28, and 3.28 mM glucose; and GOD/[email protected]
/CS/GCE (B) in the presence of 0.001 mM, 0.005, 0.01, 0.06, 0.11, 0.21, 0.31, 1.31, 2.31, 3.31 and 4.31 mM glucose in pH 7.4 PBS with 0.1 mM luminol. Inset showed linear relationship between the ECL signal intensity and the concentration of glucose.
X. Zhong et al. / Talanta 128 (2014) 9–14
limit of 0.3 μM at the signal-to-noise ratio of 3. The regression equation was I (a.u.) ¼ 3.24 103c (mM) þ617.78 with a correlation coefﬁcient of 0.9923. Compared with Fig. 3(A) the slope of GOD/ [email protected]
/CS/GCE is higher than the [email protected]
/CS/GCE that maybe own to the additional absorbing GOD outside of Aushell, which can oxidize glucose with the dissolved oxygen (O2) in the solution to form gluconolactone and produce more H2O2. Under positive potential and with the help of nanoparticles, the luminol radical anion can quickly react with those H2O2 and arise the excited state 3-aminophthalate anion to emit the stronger ECL emission. This glucose biosensor exhibited good performance due to the following reasons: (i) the GOD inside of [email protected]
still had its biological activity and [email protected]
nanoparticle had high surfaceto-volume ratio, good biocompatibility that can absorb more enzyme outside the Aushell. (ii) The [email protected]
nanoparticles assembled on the electrode could catalyze the electro-oxidization of luminol, and thus enhance the ECL intensity of luminol-H2O2 system. (iii) ECL technique has the advantages of electrochemical and luminescent techniques, such as low background disturbance, good temporal and spatial control, high sensitivity, low detection limit and so on. 3.5. Stability, reproducibility and interferences of the biosensor The reproducibility and repeatability of the sensors were performed by three assaying electrodes prepared in the same condition. A relative standard deviation (R.S.D.) was 3.9% in the presence of 0.5 mM glucose solution. A single sensor was successively tested (n ¼22) in the presence of 3.3 mM glucose (Fig. 4) with a R.S.D. of 0.8% The stability of biosensor was also the tested by monitoring its ECL response towards glucose. The prepared sensor was tested in the presence of 0.5 mM glucose solution each day, after 30 days, the response of the sensor decreased 9.6% compared to the initial response, that shows the sensors have long-term stability. Some species that usually existed and possibly interfered determination of glucose such as dopamine (DA), uric acid (UA) and p-acetamidophenol (AP) were investigated. When 0.5 mM AA, 0.5 mM UA, and 0.5 mM AP was added into 1.0 mM glucose solution, the changes in ECL signal generated from DA, UA and AP was negligible. The result revealed that the glucose biosensor has a good anti-interferent ability, which may be attributed to the enzymatic substrate-speciﬁc reaction. 3.6. Recovery experiment The applicability of the biosensor was estimated by standard addition method. Table S1 listed the recovery of different
ECL Intensity / a.u
Time/s Fig. 4. The ECL stability of GOD/[email protected]
/CS/GCE sensor to 3.31 mM glucose in pH 7.4 PBS with 0.1 mM luminol.
Table 1 Recoveries of glucose by the biosensor. Sample
1 2 3 4
50 200 500 800
5 50 50 50
56.56 7 1.9 259.3 7 6.8 534.17 22.3 827.4 7 35.5
3.4 2.6 4.2 4.3
102.8 103.7 97.0 97.3
Mean value7 standard deviation (S.D.) of three measurements.
cholesterol concentrations. The recovery rate was between 97.0% and 103.7% (See Table 1). The results proved that the biosensor had a potential for practical application.
4. Conclusions In conclusion, hollow gold nanospheres ([email protected]
) were synthesized via a method of glucose oxidase (GOD) cross-linked with glutaraldehyde as a template. An electrogenerated chemiluminescence glucose biosensor was constructed based on the [email protected]
nanoparticles. The prepared biosensor exhibited good performance that may beneﬁt from the following: ﬁrstly, the prepared hollow [email protected]
nanoparticles have a large surface area, high conductivity, good biocompatibility, which could effectively increase the loading of GOD and keep the biological activity of GOD. Thus, GOD molecules can exist inside and outside of Aushell, which could effectively amplify the ECL intensity of luminol-H2O2 system. Secondly, the Aushell assembling on the electrode can catalyze the electro-oxidization of luminol, and the stronger ECL signal was obtained in neutral aqueous solution. Such fabrication of biosensor exhibited good performance. The [email protected]
nanoparticles could have potential applications in biotechnology and clinical diagnosis.
Acknowledgments This work was supported by the National Natural Science Foundation of China (21275119, 21075100), the Ministry of Education of the People's Republic of China (Project 708073), the Nature Science Foundation of Chongqing City (CSTC-2011BA7003 and CSTC-2009BA1003), the Specialized Research Fund for the Doctoral Program of Higher Education (20100182110015), the Doctor Foundation of Southwest University (swu113029), and the Fundamental Research Funds for the Central Universities (XDJK2013C115) and (XDJK2013A008). References  A.W. Knight, G.M. Greenway, Analyst 119 (1994) 879–890.  W.J. Miao, Chem. Rev. 108 (2008) 2506–2553.  Z. Chang, J.M. Zhou, K. Zhao, N.N. Zhu, P.G. He, Y.Z. Fang, Electrochim. Acta 52 (2006) 575–580.  Y.B. Li, Z.J. Zhang, J.S. Li, H.G. Li, Y. Chen, Z.H. Liu, Talanta 84 (2011) 690–695.  S.J. Xu, Y. Liu, T.H. Wang, J.H. Li, Anal. Chem. 83 (2011) 3817–3823.  H. Dai, Y.W. Chi, X.P. Wu, Y.M. Wang, M.D. Wei, G.N. Chen, Biosens. Bioelectron. 25 (2010) 1414–1419.  Z.Y. Lin, J.J. Sun, J.H. Chen, L. Guo, Y.T. Chen, G.N. Chen, Anal. Chem. 80 (2008) 2826–2831.  L.H. Zhang, Z.A. Xu, X.P. Sun, S.J. Dong, Biosens. Bioelectron. 22 (2007) 1097–1100.  M.H. Zhang, R. Yuan, Y.Q. Chai, S.H. Chen, H.A. Zhong, C. Wang, Y.F. Cheng, Biosens. Bioelectron. 32 (2012) 288–292.  Z. Zhao, X.M. Zhou, D. Xing, Biosens. Bioelectron. 31 (2012) 299–304.  H.O. Albrecht, Z. Phys. Chem. 136 (1928) 321–330.  B. Qiu, Z.Y. Lin, J. Wang, Z.H. Chen, J.H. Chen, G.N. Chen, Talanta 78 (2009) 76–80.  T. Ren, J.Z. Xu, Y.F. Tu, S. Xu, J.J. Zhu, Electrochem. Commun. 7 (2005) 5–9.  X.M. Chen, Z.J. Lin, Z.M. Cai, X. Chen, M. Oyama, X.R. Wang, J. Nanosci. Nanotechnol. 9 (2009) 2413–2420.
X. Zhong et al. / Talanta 128 (2014) 9–14
 B. Haghighia, S. Bozorgzadeha, L. Gortonb, Sensors Actuat. B. 155 (2011) 577–583.  B. Haghighi, S. Bozorgzadeh, Anal. Chim. Acta 697 (2011) 90–97.  Q. Li, J.Y. Zheng, Y.L. Yan, Y.S. Zhao, J.N. Yao, Adv. Mater. 24 (2012) 4745–4749.  S.N. Ding, B.H. Gao, D. Shan, Y.M. Sun, S. Cosnier, Biosens. Bioelectron. 39 (2013) 342–345.  R. Cui, Y.P. Gu, L. Bao, J.Y. Zhao, B.P. Qi, Z.L. Zhang, Z.X. Xie, D.W. Pang, Anal. Chem. 84 (2012) 8932–8935.  Y.L. Cao, R. Yuan, Y.Q. Chai, Li. Mao, H. Niu, H.J. Liu, Y. Zhuo, Biosens. Bioelectron. 31 (2012) 305–309.  D.Y. Tian, C.F. Duan, W. Wang, H. Cui, Biosens. Bioelectron. 25 (2010) 2290–2295.
     
W. Wang, Y.P. Dong, H. Cui, Y. Xu, Langmuir 23 (2007) 523–529. A.J. Amali, N.H. Awwad, R.K. Rana, D. Patra, Anal. Chim. Acta 708 (2011) 75–83. D. Patra, R Aridi, K. Bouhadir, Microchim. Acta 180 (2013) 59–64. D. Patra, F Sleem, Anal. Chim. Acta 795 (2013) 60–68. D. Patra, A.J. Amali, R.K. Rana, J. Mater. Chem. 19 (2009) 4017–4021. R. Kumar, A.N. Maitra, P.K. Patanjali, P. Sharma, Biomaterials 26 (2005) 6743–6753.  J. Zhou, F. Ren, W. Wu, S.F. Zhang, X.H. Xiao, J.X. Xu, C.Z. Jiang, J. Colloid Interface Sci. 387 (2012) 47–55.  A. Manna, T. Imae, T. Yogo, K. Aoi, M. Okazaki, J. Colloid Interface Sci. 256 (2002) 297–303.